#------------------------------------------------------------------------------
#$Date: 2016-03-24 13:58:10 +0200 (Thu, 24 Mar 2016) $
#$Revision: 179647 $
#$URL: svn://www.crystallography.net/cod/cif/4/51/00/4510028.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_4510028
loop_
_publ_author_name
'Zhang, Ying'
'Shen, Jian-Qiang'
'Zheng, Li-Hua'
'Zhang, Zhi-Ming'
'Li, Yu-Xin'
'Wang, En-Bo'
_publ_section_title
;
 Four Polyoxonibate-Based Inorganic--Organic Hybrids Assembly from
 Bicapped Heteropolyoxonibate with Effective Antitumor Activity
;
_journal_issue                   1
_journal_name_full               'Crystal Growth & Design'
_journal_page_first              110
_journal_paper_doi               10.1021/cg401227g
_journal_volume                  14
_journal_year                    2014
_chemical_formula_sum            'C12 H86 Cu3 K2 N12 Na4 Nb12 O61 Si V2'
_chemical_formula_weight         2980.60
_chemical_name_systematic
; 
 ? 
;
_space_group_IT_number           12
_symmetry_cell_setting           monoclinic
_symmetry_space_group_name_Hall  '-C 2y'
_symmetry_space_group_name_H-M   'C 1 2/m 1'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 93.87(3)
_cell_angle_gamma                90.00
_cell_formula_units_Z            4
_cell_length_a                   28.942(6)
_cell_length_b                   27.294(6)
_cell_length_c                   13.568(3)
_cell_measurement_temperature    293(2)
_cell_measurement_theta_max      25.00
_cell_measurement_theta_min      3.01
_cell_volume                     10694(4)
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      293(2)
_diffrn_detector_area_resol_mean 0.01
_diffrn_measured_fraction_theta_full 0.996
_diffrn_measured_fraction_theta_max 0.996
_diffrn_measurement_device_type  'Rigaku R-AXIS RAPID IP'
_diffrn_measurement_method       Oscillation
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.1295
_diffrn_reflns_av_sigmaI/netI    0.1104
_diffrn_reflns_limit_h_max       33
_diffrn_reflns_limit_h_min       -34
_diffrn_reflns_limit_k_max       32
_diffrn_reflns_limit_k_min       -32
_diffrn_reflns_limit_l_max       16
_diffrn_reflns_limit_l_min       -14
_diffrn_reflns_number            40394
_diffrn_reflns_theta_full        25.00
_diffrn_reflns_theta_max         25.00
_diffrn_reflns_theta_min         3.01
_diffrn_standards_decay_%        none
_diffrn_standards_interval_count 0
_diffrn_standards_interval_time  0
_diffrn_standards_number         0
_exptl_absorpt_coefficient_mu    2.169
_exptl_absorpt_correction_T_max  0.8287
_exptl_absorpt_correction_T_min  0.7808
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   'ABSCOR by T.Higashi    8 March, 1995'
_exptl_crystal_colour            Purple
_exptl_crystal_density_diffrn    1.851
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       BLOCK
_exptl_crystal_F_000             5804
_exptl_crystal_size_max          0.12
_exptl_crystal_size_mid          0.11
_exptl_crystal_size_min          0.09
_refine_diff_density_max         1.526
_refine_diff_density_min         -0.981
_refine_diff_density_rms         0.190
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.053
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     621
_refine_ls_number_reflns         9603
_refine_ls_number_restraints     120
_refine_ls_restrained_S_all      1.052
_refine_ls_R_factor_all          0.1477
_refine_ls_R_factor_gt           0.0824
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.0894P)²+146.0100P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1897
_refine_ls_wR_factor_ref         0.2180
_reflns_number_gt                5494
_reflns_number_total             9603
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            cg401227g_si_005.cif
_cod_data_source_block           1
_cod_depositor_comments
;
The following automatic conversions were performed:

'_symmetry_cell_setting' value 'MONOCLINIC' changed to 'monoclinic'
according to
/usr/data/users/saulius/automatic-downloads/current/ACS/lib/dictionaries/cif_core.dic
dictionary named 'cif_core.dic' version 2.4.2 from
2011-04-26.

'_exptl_absorpt_correction_type' value 'MULTI-SCAN'
changed to 'multi-scan' according to
/usr/data/users/saulius/automatic-downloads/current/ACS/lib/dictionaries/cif_core.dic
dictionary named 'cif_core.dic' version 2.4.2 from 2011-04-26.

Automatic conversion script
Id: cif_fix_values 2281 2013-09-26 08:29:07Z andrius 
;
_cod_original_cell_volume        10693(4)
_cod_original_sg_symbol_H-M      C2/m
_cod_database_code               4510028
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, y, -z'
'x+1/2, y+1/2, z'
'-x+1/2, y+1/2, -z'
'-x, -y, -z'
'x, -y, z'
'-x+1/2, -y+1/2, -z'
'x+1/2, -y+1/2, z'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
Nb1 Nb 0.20364(4) 0.43782(4) 0.85804(9) 0.0275(3) Uani 1 1 d .
Nb2 Nb 0.32758(4) 0.43807(5) 0.95671(10) 0.0333(3) Uani 1 1 d .
Nb3 Nb 0.15653(4) 0.43150(5) 1.22366(9) 0.0294(3) Uani 1 1 d .
Nb4 Nb 0.12154(5) 0.5000 0.98394(13) 0.0310(4) Uani 1 2 d S
Nb5 Nb 0.23783(5) 0.36840(4) 1.09717(10) 0.0359(3) Uani 1 1 d .
Nb6 Nb 0.26897(4) 0.43126(5) 1.31312(9) 0.0321(3) Uani 1 1 d .
Nb7 Nb 0.35977(6) 0.5000 1.17415(15) 0.0389(5) Uani 1 2 d S
Cu1 Cu 0.22495(7) 0.23872(7) 1.18133(15) 0.0499(5) Uani 1 1 d .
Cu2 Cu 0.01518(8) 0.5000 0.8120(2) 0.0465(7) Uani 1 2 d S
V1 V 0.14354(14) 0.39365(16) 1.0120(3) 0.0267(10) Uani 0.50 1 d P
V2 V 0.33577(16) 0.39262(19) 1.1638(4) 0.0373(12) Uani 0.50 1 d P
Si1 Si 0.23946(17) 0.5000 1.0886(4) 0.0267(11) Uani 1 2 d S
K1 K 0.18437(19) 0.5000 1.4617(4) 0.0595(14) Uani 1 2 d S
K2 K 0.2916(2) 0.5000 0.7096(4) 0.0649(16) Uani 1 2 d S
Na1 Na 0.0000 0.0641(5) 1.0000 0.077(4) Uani 0.84 2 d SPU
Na2 Na 0.0385(6) 0.2818(6) 0.9393(16) 0.076(5) Uani 0.42 1 d P
Na3 Na 0.1303(6) 0.3733(7) 0.6148(13) 0.075(5) Uani 0.43 1 d P
Na4 Na 0.0710(6) 0.3229(7) 1.3398(17) 0.077(6) Uani 0.38 1 d P
Na5 Na 0.2098(7) 0.1486(8) 1.2738(15) 0.065(5) Uani 0.35 1 d PU
O1 O 0.1278(3) 0.4501(3) 1.0894(6) 0.028(2) Uani 1 1 d .
O2 O 0.2061(3) 0.3900(3) 0.9714(6) 0.0238(19) Uani 1 1 d .
O3 O 0.1538(4) 0.5000 1.2607(9) 0.034(3) Uani 1 2 d S
O4 O 0.2937(4) 0.5000 1.0580(9) 0.029(3) Uani 1 2 d S
O5 O 0.2052(4) 0.5000 0.9874(8) 0.026(3) Uani 1 2 d S
O6 O 0.0609(4) 0.5000 0.9605(10) 0.039(3) Uani 1 2 d S
O7 O 0.2709(3) 0.4410(3) 0.8731(7) 0.031(2) Uani 1 1 d .
O8 O 0.2296(3) 0.4505(3) 1.1534(6) 0.0262(19) Uani 1 1 d .
O9 O 0.2967(3) 0.3900(3) 1.0441(7) 0.032(2) Uani 1 1 d .
O10 O 0.2408(3) 0.3049(3) 1.0748(7) 0.035(2) Uani 1 1 d .
O11 O 0.3497(4) 0.5000 0.9049(10) 0.034(3) Uani 1 2 d S
O12 O 0.2000(4) 0.5000 0.7854(9) 0.032(3) Uani 1 2 d S
O13 O 0.3271(3) 0.4498(3) 1.2482(7) 0.034(2) Uani 1 1 d .
O14 O 0.1755(3) 0.3706(3) 1.1526(7) 0.037(2) Uani 1 1 d .
O15 O 0.1967(3) 0.3959(4) 0.7583(7) 0.037(2) Uani 1 1 d .
O16 O 0.2035(3) 0.4172(3) 1.3313(6) 0.033(2) Uani 1 1 d .
O17 O 0.1069(3) 0.4096(4) 1.2766(7) 0.042(2) Uani 1 1 d .
O18 O 0.3604(3) 0.3959(4) 0.8895(8) 0.049(3) Uani 1 1 d .
O19 O 0.1374(3) 0.4466(3) 0.8928(7) 0.036(2) Uani 1 1 d .
O20 O 0.3709(3) 0.4473(4) 1.0799(8) 0.047(3) Uani 1 1 d .
O21 O 0.2940(3) 0.4070(4) 1.4264(7) 0.043(2) Uani 1 1 d .
O22 O 0.2728(3) 0.3705(3) 1.2280(7) 0.039(2) Uani 1 1 d .
O23 O 0.4150(4) 0.5000 1.2431(12) 0.051(4) Uani 1 2 d S
O24 O 0.2619(4) 0.5000 1.3456(9) 0.029(3) Uani 1 2 d S
O25 O 0.1061(4) 0.3524(4) 0.9810(9) 0.060(3) Uani 1 1 d .
O26 O 0.3692(4) 0.3573(5) 1.1915(11) 0.081(4) Uani 1 1 d .
O1W O 0.2375(4) 0.4377(5) 1.5864(10) 0.076(4) Uani 1 1 d U
O2W O 0.1321(7) 0.5000 1.6316(16) 0.092(6) Uani 1 2 d SU
O3W O 0.3340(12) 0.5000 0.528(3) 0.145(13) Uiso 0.80 2 d SP
O4W O 0.1838(6) 0.3389(7) 1.4500(13) 0.121(6) Uani 1 1 d U
O27W O 0.0718(9) 0.2909(11) 0.609(2) 0.104(9) Uani 0.58 1 d PU
O26W O 0.0910(11) 0.4415(12) 1.459(2) 0.104(10) Uani 0.52 1 d PU
O25W O 0.2792(10) 0.3189(11) 1.527(2) 0.103(9) Uani 0.58 1 d PU
O24W O 0.0000 0.3330(18) 1.5000 0.110(15) Uani 0.52 2 d SPU
O23W O 0.1403(13) 0.2502(15) 1.442(3) 0.129(13) Uani 0.49 1 d PU
O22W O 0.0022(11) 0.2721(12) 1.247(2) 0.102(10) Uani 0.51 1 d PU
O21W O 0.042(2) 0.0000 1.033(5) 0.16(2) Uani 0.50 2 d SPU
O20W O -0.0533(16) 0.5000 0.644(4) 0.114(16) Uani 0.50 2 d SPU
O19W O 0.398(2) 0.443(3) 1.423(6) 0.13(3) Uani 0.25 1 d PU
O18W O 0.415(2) 0.5000 0.763(6) 0.19(3) Uani 0.50 2 d SPU
O17W O 0.0123(17) 0.5714(17) 0.527(4) 0.115(18) Uani 0.35 1 d PU
O16W O 0.4514(16) 0.366(2) 0.896(4) 0.087(15) Uani 0.28 1 d PU
O15W O 0.048(2) 0.124(2) 1.006(5) 0.106(19) Uani 0.27 1 d PU
O14W O 0.145(2) 0.098(3) 1.310(5) 0.12(2) Uani 0.26 1 d PU
O13W O 0.057(3) 0.183(3) 0.887(6) 0.15(3) Uani 0.25 1 d PU
O10W O 0.044(3) 0.192(3) 1.321(6) 0.14(3) Uiso 0.25 1 d P
C1 C 0.0021(6) 0.5997(7) 0.8632(14) 0.067(5) Uani 1 1 d .
H1A H 0.0239 0.6004 0.9208 0.080 Uiso 1 1 calc R
H1B H -0.0185 0.6275 0.8660 0.080 Uiso 1 1 calc R
C2 C 0.3229(6) 0.2342(7) 1.1970(13) 0.063(5) Uani 1 1 d .
H2A H 0.3275 0.2648 1.1626 0.076 Uiso 1 1 calc R
H2B H 0.3513 0.2154 1.1976 0.076 Uiso 1 1 calc R
C3 C 0.1264(7) 0.2474(8) 1.1564(18) 0.085(7) Uani 1 1 d .
H3A H 0.1009 0.2705 1.1507 0.103 Uiso 1 1 calc R
H3B H 0.1158 0.2176 1.1866 0.103 Uiso 1 1 calc R
C4 C 0.1431(6) 0.2365(7) 1.0559(16) 0.071(6) Uani 1 1 d .
H4A H 0.1200 0.2177 1.0170 0.085 Uiso 1 1 calc R
H4B H 0.1488 0.2667 1.0212 0.085 Uiso 1 1 calc R
C5 C 0.3104(7) 0.2440(7) 1.3001(13) 0.075(6) Uani 1 1 d .
H5A H 0.3089 0.2135 1.3365 0.089 Uiso 1 1 calc R
H5B H 0.3334 0.2650 1.3340 0.089 Uiso 1 1 calc R
C6 C 0.0269(6) 0.6011(8) 0.7725(16) 0.079(7) Uani 1 1 d .
H6A H 0.0489 0.6280 0.7763 0.095 Uiso 1 1 calc R
H6B H 0.0050 0.6070 0.7164 0.095 Uiso 1 1 calc R
N1 N 0.2845(4) 0.2065(5) 1.1473(10) 0.049(3) Uani 1 1 d .
H1C H 0.2852 0.1752 1.1680 0.059 Uiso 1 1 calc R
H1D H 0.2868 0.2068 1.0815 0.059 Uiso 1 1 calc R
N2 N 0.1658(5) 0.2686(5) 1.2173(11) 0.064(4) Uani 1 1 d .
H2C H 0.1619 0.2631 1.2817 0.077 Uiso 1 1 calc R
H2D H 0.1667 0.3012 1.2078 0.077 Uiso 1 1 calc R
N3 N -0.0240(4) 0.5543(5) 0.8604(10) 0.049(3) Uani 1 1 d .
H3C H -0.0497 0.5577 0.8199 0.059 Uiso 1 1 calc R
H3D H -0.0326 0.5472 0.9213 0.059 Uiso 1 1 calc R
N4 N 0.1860(4) 0.2083(5) 1.0711(10) 0.052(4) Uani 1 1 d .
H4C H 0.2013 0.2085 1.0155 0.062 Uiso 1 1 calc R
H4D H 0.1795 0.1771 1.0860 0.062 Uiso 1 1 calc R
N5 N 0.2646(6) 0.2684(5) 1.2936(10) 0.067(4) Uani 1 1 d .
H5C H 0.2681 0.3007 1.2832 0.080 Uiso 1 1 calc R
H5D H 0.2508 0.2644 1.3506 0.080 Uiso 1 1 calc R
N6 N 0.0521(4) 0.5540(6) 0.7571(11) 0.064(4) Uani 1 1 d .
H6C H 0.0805 0.5550 0.7882 0.077 Uiso 1 1 calc R
H6D H 0.0551 0.5490 0.6923 0.077 Uiso 1 1 calc R
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Nb Nb -2.0727 0.6215 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Cu Cu 0.3201 1.2651 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Si Si 0.0817 0.0704 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
K K 0.2009 0.2494 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
V V 0.3005 0.5294 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Na Na 0.0362 0.0249 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
O15 Nb1 O7 99.8(4) . .
O15 Nb1 O12 100.1(4) . .
O7 Nb1 O12 91.9(4) . .
O15 Nb1 O2 99.2(4) . .
O7 Nb1 O2 88.1(3) . .
O12 Nb1 O2 160.4(4) . .
O15 Nb1 O19 101.2(4) . .
O7 Nb1 O19 158.3(4) . .
O12 Nb1 O19 89.7(5) . .
O2 Nb1 O19 83.3(4) . .
O15 Nb1 O5 173.5(4) . .
O7 Nb1 O5 85.6(4) . .
O12 Nb1 O5 76.0(4) . .
O2 Nb1 O5 84.5(3) . .
O19 Nb1 O5 73.8(4) . .
O15 Nb1 V1 103.1(3) . .
O7 Nb1 V1 123.9(3) . .
O12 Nb1 V1 132.2(4) . .
O2 Nb1 V1 38.3(2) . .
O19 Nb1 V1 45.1(3) . .
O5 Nb1 V1 76.5(2) . .
O15 Nb1 K2 85.9(3) . .
O7 Nb1 K2 47.6(3) . .
O12 Nb1 K2 49.8(4) . .
O2 Nb1 K2 135.4(2) . .
O19 Nb1 K2 139.5(3) . .
O5 Nb1 K2 95.2(2) . .
V1 Nb1 K2 169.32(13) . .
O18 Nb2 O7 100.8(4) . .
O18 Nb2 O11 100.1(5) . .
O7 Nb2 O11 92.2(5) . .
O18 Nb2 O9 98.8(4) . .
O7 Nb2 O9 88.8(4) . .
O11 Nb2 O9 160.5(4) . .
O18 Nb2 O20 100.4(4) . .
O7 Nb2 O20 158.2(4) . .
O11 Nb2 O20 89.4(5) . .
O9 Nb2 O20 82.6(4) . .
O18 Nb2 O4 171.7(4) . .
O7 Nb2 O4 86.8(4) . .
O11 Nb2 O4 75.9(4) . .
O9 Nb2 O4 84.7(3) . .
O20 Nb2 O4 72.5(4) . .
O18 Nb2 V2 101.4(4) . .
O7 Nb2 V2 124.4(3) . .
O11 Nb2 V2 132.2(4) . .
O9 Nb2 V2 37.6(3) . .
O20 Nb2 V2 45.0(3) . .
O4 Nb2 V2 76.8(3) . .
O18 Nb2 K2 87.7(4) . .
O7 Nb2 K2 45.5(3) . .
O11 Nb2 K2 51.7(4) . .
O9 Nb2 K2 134.1(3) . .
O20 Nb2 K2 141.1(3) . .
O4 Nb2 K2 95.3(3) . .
V2 Nb2 K2 168.25(13) . .
O17 Nb3 O3 100.0(5) . .
O17 Nb3 O16 100.0(4) . .
O3 Nb3 O16 92.1(5) . .
O17 Nb3 O1 99.0(4) . .
O3 Nb3 O1 88.3(4) . .
O16 Nb3 O1 160.7(3) . .
O17 Nb3 O14 99.9(4) . .
O3 Nb3 O14 159.5(5) . .
O16 Nb3 O14 89.7(4) . .
O1 Nb3 O14 83.4(4) . .
O17 Nb3 O8 172.1(4) . .
O3 Nb3 O8 87.1(4) . .
O16 Nb3 O8 76.0(3) . .
O1 Nb3 O8 84.8(3) . .
O14 Nb3 O8 73.5(3) . .
O17 Nb3 V1 102.6(3) . .
O3 Nb3 V1 124.5(4) . .
O16 Nb3 V1 131.8(3) . .
O1 Nb3 V1 38.5(3) . .
O14 Nb3 V1 44.9(3) . .
O8 Nb3 V1 76.0(2) . .
O17 Nb3 K1 87.2(4) . .
O3 Nb3 K1 46.4(4) . .
O16 Nb3 K1 50.6(3) . .
O1 Nb3 K1 134.5(3) . .
O14 Nb3 K1 140.3(3) . .
O8 Nb3 K1 95.1(2) . .
V1 Nb3 K1 168.36(11) . .
O6 Nb4 O1 99.9(4) . 6_565
O6 Nb4 O1 99.9(4) . .
O1 Nb4 O1 87.2(5) 6_565 .
O6 Nb4 O19 99.0(4) . 6_565
O1 Nb4 O19 86.1(4) 6_565 6_565
O1 Nb4 O19 160.7(4) . 6_565
O6 Nb4 O19 99.0(4) . .
O1 Nb4 O19 160.7(3) 6_565 .
O1 Nb4 O19 86.1(4) . .
O19 Nb4 O19 94.5(6) 6_565 .
O6 Nb4 O5 170.8(5) . .
O1 Nb4 O5 86.7(3) 6_565 .
O1 Nb4 O5 86.7(3) . .
O19 Nb4 O5 74.9(3) 6_565 .
O19 Nb4 O5 74.9(3) . .
O6 Nb4 V1 102.93(9) . 6_565
O1 Nb4 V1 39.7(3) 6_565 6_565
O1 Nb4 V1 124.7(3) . 6_565
O19 Nb4 V1 46.4(3) 6_565 6_565
O19 Nb4 V1 137.4(3) . 6_565
O5 Nb4 V1 78.07(9) . 6_565
O6 Nb4 V1 102.93(9) . .
O1 Nb4 V1 124.7(3) 6_565 .
O1 Nb4 V1 39.7(3) . .
O19 Nb4 V1 137.4(3) 6_565 .
O19 Nb4 V1 46.4(3) . .
O5 Nb4 V1 78.07(9) . .
V1 Nb4 V1 152.17(17) 6_565 .
O10 Nb5 O2 99.8(4) . .
O10 Nb5 O9 100.2(4) . .
O2 Nb5 O9 87.6(3) . .
O10 Nb5 O22 98.9(4) . .
O2 Nb5 O22 161.0(4) . .
O9 Nb5 O22 85.3(4) . .
O10 Nb5 O14 98.6(4) . .
O2 Nb5 O14 86.4(4) . .
O9 Nb5 O14 161.0(4) . .
O22 Nb5 O14 94.7(4) . .
O10 Nb5 O8 170.5(4) . .
O2 Nb5 O8 86.9(3) . .
O9 Nb5 O8 86.8(3) . .
O22 Nb5 O8 75.1(3) . .
O14 Nb5 O8 74.9(3) . .
O10 Nb5 V1 102.4(3) . .
O2 Nb5 V1 39.9(2) . .
O9 Nb5 V1 125.3(3) . .
O22 Nb5 V1 137.8(3) . .
O14 Nb5 V1 46.5(3) . .
O8 Nb5 V1 78.3(2) . .
O10 Nb5 V2 102.3(3) . .
O2 Nb5 V2 124.9(2) . .
O9 Nb5 V2 39.1(3) . .
O22 Nb5 V2 46.1(3) . .
O14 Nb5 V2 137.7(3) . .
O8 Nb5 V2 79.0(2) . .
V1 Nb5 V2 153.26(13) . .
O21 Nb6 O24 101.9(5) . .
O21 Nb6 O16 99.1(4) . .
O24 Nb6 O16 92.5(4) . .
O21 Nb6 O13 99.7(4) . .
O24 Nb6 O13 87.7(4) . .
O16 Nb6 O13 160.8(4) . .
O21 Nb6 O22 98.8(4) . .
O24 Nb6 O22 158.5(4) . .
O16 Nb6 O22 90.1(4) . .
O13 Nb6 O22 83.0(4) . .
O21 Nb6 O8 170.3(4) . .
O24 Nb6 O8 86.8(4) . .
O16 Nb6 O8 75.9(3) . .
O13 Nb6 O8 84.9(3) . .
O22 Nb6 O8 73.1(3) . .
O21 Nb6 V2 101.8(3) . .
O24 Nb6 V2 124.1(4) . .
O16 Nb6 V2 132.0(3) . .
O13 Nb6 V2 38.7(3) . .
O22 Nb6 V2 44.3(3) . .
O8 Nb6 V2 76.4(2) . .
O21 Nb6 K1 87.9(3) . .
O24 Nb6 K1 46.9(4) . .
O16 Nb6 K1 50.5(3) . .
O13 Nb6 K1 134.4(3) . .
O22 Nb6 K1 140.6(3) . .
O8 Nb6 K1 95.0(2) . .
V2 Nb6 K1 168.63(12) . .
O23 Nb7 O20 99.2(4) . 6_565
O23 Nb7 O20 99.2(4) . .
O20 Nb7 O20 94.1(7) 6_565 .
O23 Nb7 O13 100.1(4) . .
O20 Nb7 O13 160.5(4) 6_565 .
O20 Nb7 O13 85.9(4) . .
O23 Nb7 O13 100.1(4) . 6_565
O20 Nb7 O13 85.9(4) 6_565 6_565
O20 Nb7 O13 160.5(4) . 6_565
O13 Nb7 O13 87.7(5) . 6_565
O23 Nb7 O4 170.2(6) . .
O20 Nb7 O4 74.4(3) 6_565 .
O20 Nb7 O4 74.4(3) . .
O13 Nb7 O4 86.9(3) . .
O13 Nb7 O4 86.9(3) 6_565 .
O23 Nb7 V2 102.62(11) . .
O20 Nb7 V2 136.8(3) 6_565 .
O20 Nb7 V2 46.0(3) . .
O13 Nb7 V2 39.9(3) . .
O13 Nb7 V2 125.5(3) 6_565 .
O4 Nb7 V2 78.35(11) . .
O23 Nb7 V2 102.62(11) . 6_565
O20 Nb7 V2 46.0(3) 6_565 6_565
O20 Nb7 V2 136.8(3) . 6_565
O13 Nb7 V2 125.5(3) . 6_565
O13 Nb7 V2 39.9(3) 6_565 6_565
O4 Nb7 V2 78.35(11) . 6_565
V2 Nb7 V2 153.16(19) . 6_565
N2 Cu1 N4 84.3(6) . .
N2 Cu1 N1 178.2(6) . .
N4 Cu1 N1 95.5(5) . .
N2 Cu1 N5 96.0(7) . .
N4 Cu1 N5 179.1(6) . .
N1 Cu1 N5 84.1(6) . .
N2 Cu1 O10 92.4(5) . .
N4 Cu1 O10 89.0(5) . .
N1 Cu1 O10 89.4(4) . .
N5 Cu1 O10 91.8(5) . .
N2 Cu1 Na5 95.0(6) . .
N4 Cu1 Na5 82.7(6) . .
N1 Cu1 Na5 83.2(5) . .
N5 Cu1 Na5 96.4(6) . .
O10 Cu1 Na5 168.3(5) . .
N6 Cu2 N6 95.3(9) 6_565 .
N6 Cu2 N3 177.0(6) 6_565 .
N6 Cu2 N3 84.5(6) . .
N6 Cu2 N3 84.5(6) 6_565 6_565
N6 Cu2 N3 177.0(6) . 6_565
N3 Cu2 N3 95.5(8) . 6_565
N6 Cu2 O6 92.1(5) 6_565 .
N6 Cu2 O6 92.1(5) . .
N3 Cu2 O6 91.0(4) . .
N3 Cu2 O6 91.0(4) 6_565 .
O25 V1 O2 121.4(6) . .
O25 V1 O1 121.5(6) . .
O2 V1 O1 117.1(4) . .
O25 V1 O14 105.6(5) . .
O2 V1 O14 83.3(4) . .
O1 V1 O14 81.6(4) . .
O25 V1 O19 104.7(5) . .
O2 V1 O19 81.6(4) . .
O1 V1 O19 82.2(4) . .
O14 V1 O19 149.7(4) . .
O25 V1 Nb5 121.8(5) . .
O2 V1 Nb5 40.9(3) . .
O1 V1 Nb5 102.5(3) . .
O14 V1 Nb5 42.4(2) . .
O19 V1 Nb5 118.1(3) . .
O25 V1 Nb4 121.0(5) . .
O2 V1 Nb4 102.1(3) . .
O1 V1 Nb4 40.6(3) . .
O14 V1 Nb4 118.1(3) . .
O19 V1 Nb4 41.6(3) . .
Nb5 V1 Nb4 117.17(14) . .
O25 V1 Nb3 121.6(5) . .
O2 V1 Nb3 103.2(3) . .
O1 V1 Nb3 40.4(3) . .
O14 V1 Nb3 41.2(3) . .
O19 V1 Nb3 118.4(3) . .
Nb5 V1 Nb3 70.17(10) . .
Nb4 V1 Nb3 78.62(12) . .
O25 V1 Nb1 120.3(5) . .
O2 V1 Nb1 40.3(3) . .
O1 V1 Nb1 102.9(3) . .
O14 V1 Nb1 119.4(3) . .
O19 V1 Nb1 41.3(2) . .
Nb5 V1 Nb1 78.88(11) . .
Nb4 V1 Nb1 69.89(10) . .
Nb3 V1 Nb1 118.04(14) . .
O26 V2 O9 124.0(7) . .
O26 V2 O13 120.3(7) . .
O9 V2 O13 115.6(5) . .
O26 V2 O22 106.7(7) . .
O9 V2 O22 82.2(4) . .
O13 V2 O22 80.9(4) . .
O26 V2 O20 105.8(7) . .
O9 V2 O20 81.5(4) . .
O13 V2 O20 80.9(4) . .
O22 V2 O20 147.4(4) . .
O26 V2 Nb5 123.6(6) . .
O9 V2 Nb5 40.7(3) . .
O13 V2 Nb5 101.3(3) . .
O22 V2 Nb5 41.5(3) . .
O20 V2 Nb5 117.5(3) . .
O26 V2 Nb7 120.3(6) . .
O9 V2 Nb7 101.3(3) . .
O13 V2 Nb7 40.3(3) . .
O22 V2 Nb7 116.9(3) . .
O20 V2 Nb7 40.6(3) . .
Nb5 V2 Nb7 116.10(17) . .
O26 V2 Nb2 122.2(7) . .
O9 V2 Nb2 40.0(3) . .
O13 V2 Nb2 102.0(3) . .
O22 V2 Nb2 117.9(3) . .
O20 V2 Nb2 41.5(3) . .
Nb5 V2 Nb2 78.42(13) . .
Nb7 V2 Nb2 69.65(12) . .
O26 V2 Nb6 120.9(7) . .
O9 V2 Nb6 102.1(3) . .
O13 V2 Nb6 39.9(3) . .
O22 V2 Nb6 41.1(3) . .
O20 V2 Nb6 116.5(3) . .
Nb5 V2 Nb6 69.53(11) . .
Nb7 V2 Nb6 77.84(13) . .
Nb2 V2 Nb6 116.82(16) . .
O5 Si1 O8 109.3(4) . 6_565
O5 Si1 O8 109.3(4) . .
O8 Si1 O8 110.2(7) 6_565 .
O5 Si1 O4 108.8(7) . .
O8 Si1 O4 109.7(4) 6_565 .
O8 Si1 O4 109.7(4) . .
O1W K1 O1W 75.2(6) 6_565 .
O1W K1 O3 135.6(3) 6_565 .
O1W K1 O3 135.6(3) . .
O1W K1 O24 84.9(4) 6_565 .
O1W K1 O24 84.9(4) . .
O3 K1 O24 70.7(4) . .
O1W K1 O2W 79.0(4) 6_565 .
O1W K1 O2W 79.0(4) . .
O3 K1 O2W 129.6(5) . .
O24 K1 O2W 159.7(5) . .
O1W K1 O16 77.2(3) 6_565 6_565
O1W K1 O16 135.6(4) . 6_565
O3 K1 O16 58.4(2) . 6_565
O24 K1 O16 58.5(2) . 6_565
O2W K1 O16 128.3(2) . 6_565
O1W K1 O16 135.6(4) 6_565 .
O1W K1 O16 77.2(3) . .
O3 K1 O16 58.4(2) . .
O24 K1 O16 58.5(2) . .
O2W K1 O16 128.3(2) . .
O16 K1 O16 100.2(4) 6_565 .
O1W K1 O26W 139.3(7) 6_565 .
O1W K1 O26W 97.9(7) . .
O3 K1 O26W 76.9(6) . .
O24 K1 O26W 135.1(6) . .
O2W K1 O26W 60.3(7) . .
O16 K1 O26W 125.4(7) 6_565 .
O16 K1 O26W 78.3(6) . .
O1W K1 O26W 97.9(7) 6_565 6_565
O1W K1 O26W 139.3(7) . 6_565
O3 K1 O26W 76.9(6) . 6_565
O24 K1 O26W 135.1(6) . 6_565
O2W K1 O26W 60.3(7) . 6_565
O16 K1 O26W 78.3(6) 6_565 6_565
O16 K1 O26W 125.4(7) . 6_565
O26W K1 O26W 61.3(12) . 6_565
O1W K1 Nb3 154.1(3) 6_565 .
O1W K1 Nb3 107.1(3) . .
O3 K1 Nb3 29.98(6) . .
O24 K1 Nb3 69.8(2) . .
O2W K1 Nb3 126.9(3) . .
O16 K1 Nb3 84.5(2) 6_565 .
O16 K1 Nb3 31.04(19) . .
O26W K1 Nb3 66.6(6) . .
O26W K1 Nb3 96.2(6) 6_565 .
O1W K1 Nb3 107.1(3) 6_565 6_565
O1W K1 Nb3 154.1(3) . 6_565
O3 K1 Nb3 29.98(6) . 6_565
O24 K1 Nb3 69.8(2) . 6_565
O2W K1 Nb3 126.9(3) . 6_565
O16 K1 Nb3 31.04(19) 6_565 6_565
O16 K1 Nb3 84.5(2) . 6_565
O26W K1 Nb3 96.2(6) . 6_565
O26W K1 Nb3 66.6(6) 6_565 6_565
Nb3 K1 Nb3 59.44(9) . 6_565
O1W K1 Nb6 70.7(3) 6_565 6_565
O1W K1 Nb6 106.0(3) . 6_565
O3 K1 Nb6 69.8(2) . 6_565
O24 K1 Nb6 30.07(6) . 6_565
O2W K1 Nb6 146.5(2) . 6_565
O16 K1 Nb6 30.99(17) 6_565 6_565
O16 K1 Nb6 84.6(2) . 6_565
O26W K1 Nb6 146.7(6) . 6_565
O26W K1 Nb6 109.2(6) 6_565 6_565
Nb3 K1 Nb6 84.14(11) . 6_565
Nb3 K1 Nb6 53.48(7) 6_565 6_565
O1W K2 O1W 75.1(6) 1_554 6_564
O1W K2 O3W 74.7(6) 1_554 .
O1W K2 O3W 74.7(6) 6_564 .
O1W K2 O7 89.0(3) 1_554 .
O1W K2 O7 132.4(4) 6_564 .
O3W K2 O7 144.0(3) . .
O1W K2 O7 132.4(4) 1_554 6_565
O1W K2 O7 89.0(3) 6_564 6_565
O3W K2 O7 144.0(3) . 6_565
O7 K2 O7 69.1(4) . 6_565
O1W K2 O12 74.0(3) 1_554 .
O1W K2 O12 74.0(3) 6_564 .
O3W K2 O12 140.2(8) . .
O7 K2 O12 58.5(3) . .
O7 K2 O12 58.5(3) 6_565 .
O1W K2 O11 141.0(3) 1_554 .
O1W K2 O11 141.0(3) 6_564 .
O3W K2 O11 120.8(8) . .
O7 K2 O11 56.8(3) . .
O7 K2 O11 56.8(3) 6_565 .
O12 K2 O11 99.0(4) . .
O1W K2 O14W 138.3(13) 1_554 4_557
O1W K2 O14W 75.4(13) 6_564 4_557
O3W K2 O14W 69.6(13) . 4_557
O7 K2 O14W 132.6(13) . 4_557
O7 K2 O14W 75.4(12) 6_565 4_557
O12 K2 O14W 124.0(12) . 4_557
O11 K2 O14W 77.8(13) . 4_557
O1W K2 O14W 75.4(13) 1_554 7_557
O1W K2 O14W 138.3(13) 6_564 7_557
O3W K2 O14W 69.6(13) . 7_557
O7 K2 O14W 75.4(12) . 7_557
O7 K2 O14W 132.6(13) 6_565 7_557
O12 K2 O14W 124.0(12) . 7_557
O11 K2 O14W 77.8(13) . 7_557
O14W K2 O14W 110(2) 4_557 7_557
O1W K2 Nb1 70.9(3) 1_554 .
O1W K2 Nb1 102.9(3) 6_564 .
O3W K2 Nb1 144.8(5) . .
O7 K2 Nb1 30.45(18) . .
O7 K2 Nb1 69.5(2) 6_565 .
O12 K2 Nb1 31.04(13) . .
O11 K2 Nb1 83.6(2) . .
O14W K2 Nb1 144.9(12) 4_557 .
O14W K2 Nb1 94.5(12) 7_557 .
O1W K2 Nb1 102.9(3) 1_554 6_565
O1W K2 Nb1 70.9(3) 6_564 6_565
O3W K2 Nb1 144.8(5) . 6_565
O7 K2 Nb1 69.5(2) . 6_565
O7 K2 Nb1 30.45(18) 6_565 6_565
O12 K2 Nb1 31.04(13) . 6_565
O11 K2 Nb1 83.6(2) . 6_565
O14W K2 Nb1 94.5(12) 4_557 6_565
O14W K2 Nb1 144.9(12) 7_557 6_565
Nb1 K2 Nb1 53.72(9) . 6_565
O1W K2 Nb2 154.3(3) 1_554 6_565
O1W K2 Nb2 111.3(3) 6_564 6_565
O3W K2 Nb2 130.9(6) . 6_565
O7 K2 Nb2 68.0(2) . 6_565
O7 K2 Nb2 29.05(18) 6_565 6_565
O12 K2 Nb2 83.7(3) . 6_565
O11 K2 Nb2 30.34(12) . 6_565
O14W K2 Nb2 65.7(12) 4_557 6_565
O14W K2 Nb2 108.1(12) 7_557 6_565
Nb1 K2 Nb2 83.36(11) . 6_565
Nb1 K2 Nb2 59.07(8) 6_565 6_565
O15W Na1 O15W 80(3) . 2_557
O15W Na1 O21W 169(2) . 5_557
O15W Na1 O21W 105(2) 2_557 5_557
O15W Na1 O21W 105(2) . .
O15W Na1 O21W 169(2) 2_557 .
O21W Na1 O21W 72(3) 5_557 .
O15W Na1 O16W 29.5(19) . 7_557
O15W Na1 O16W 78.0(19) 2_557 7_557
O21W Na1 O16W 161(2) 5_557 7_557
O21W Na1 O16W 101.3(18) . 7_557
O15W Na1 O16W 78.0(19) . 8_455
O15W Na1 O16W 29.5(19) 2_557 8_455
O21W Na1 O16W 101.3(18) 5_557 8_455
O21W Na1 O16W 161(2) . 8_455
O16W Na1 O16W 90(2) 7_557 8_455
O15W Na1 Na1 139.9(17) . 5_557
O15W Na1 Na1 139.9(17) 2_557 5_557
O21W Na1 Na1 36.2(13) 5_557 5_557
O21W Na1 Na1 36.2(13) . 5_557
O16W Na1 Na1 134.9(12) 7_557 5_557
O16W Na1 Na1 134.9(12) 8_455 5_557
O22W Na2 O25 120.6(10) 2_557 .
O22W Na2 O13W 75.7(19) 2_557 .
O25 Na2 O13W 124.7(17) . .
O22W Na2 Na2 103.3(10) 2_557 2_557
O25 Na2 Na2 116.7(8) . 2_557
O13W Na2 Na2 107.9(17) . 2_557
O15 Na3 O27W 126.7(9) . .
O15 Na3 O4W 103.5(7) . 1_554
O27W Na3 O4W 94.0(9) . 1_554
O15 Na3 O26W 125.8(9) . 1_554
O27W Na3 O26W 106.2(10) . 1_554
O4W Na3 O26W 81.7(8) 1_554 1_554
O15 Na3 K1 84.4(5) . 1_554
O27W Na3 K1 148.5(8) . 1_554
O4W Na3 K1 70.7(5) 1_554 1_554
O26W Na3 K1 45.7(6) 1_554 1_554
O22W Na4 O17 125.9(11) . .
O14W Na5 Cu1 138.0(19) . .
O14W Na5 O25W 91.6(19) . 7_558
Cu1 Na5 O25W 98.1(9) . 7_558
O14W Na5 K2 53.1(18) . 7_557
Cu1 Na5 K2 154.3(7) . 7_557
O25W Na5 K2 105.0(8) 7_558 7_557
V1 O1 Nb4 99.7(4) . .
V1 O1 Nb3 101.1(4) . .
Nb4 O1 Nb3 147.2(5) . .
V1 O2 Nb5 99.2(4) . .
V1 O2 Nb1 101.5(4) . .
Nb5 O2 Nb1 147.6(4) . .
Nb3 O3 Nb3 149.2(7) 6_565 .
Nb3 O3 K1 103.6(4) 6_565 .
Nb3 O3 K1 103.6(4) . .
Si1 O4 Nb7 124.4(7) . .
Si1 O4 Nb2 124.7(4) . 6_565
Nb7 O4 Nb2 92.2(3) . 6_565
Si1 O4 Nb2 124.7(4) . .
Nb7 O4 Nb2 92.2(3) . .
Nb2 O4 Nb2 88.3(4) 6_565 .
Si1 O5 Nb4 124.4(6) . .
Si1 O5 Nb1 125.7(4) . .
Nb4 O5 Nb1 90.9(3) . .
Si1 O5 Nb1 125.7(4) . 6_565
Nb4 O5 Nb1 90.9(3) . 6_565
Nb1 O5 Nb1 88.1(4) . 6_565
Nb4 O6 Cu2 130.9(7) . .
Nb2 O7 Nb1 149.7(5) . .
Nb2 O7 K2 105.5(4) . .
Nb1 O7 K2 101.9(4) . .
Si1 O8 Nb5 125.1(5) . .
Si1 O8 Nb3 124.8(4) . .
Nb5 O8 Nb3 92.0(3) . .
Si1 O8 Nb6 124.3(5) . .
Nb5 O8 Nb6 91.8(3) . .
Nb3 O8 Nb6 88.4(3) . .
V2 O9 Nb5 100.1(4) . .
V2 O9 Nb2 102.3(4) . .
Nb5 O9 Nb2 146.3(5) . .
Nb5 O10 Cu1 129.0(5) . .
Nb2 O11 Nb2 119.6(6) 6_565 .
Nb2 O11 K2 97.9(4) 6_565 .
Nb2 O11 K2 97.9(4) . .
Nb1 O12 Nb1 119.8(6) 6_565 .
Nb1 O12 K2 99.1(4) 6_565 .
Nb1 O12 K2 99.1(4) . .
V2 O13 Nb7 99.8(4) . .
V2 O13 Nb6 101.5(4) . .
Nb7 O13 Nb6 147.0(5) . .
Nb5 O14 Nb3 119.0(4) . .
Nb5 O14 V1 91.1(4) . .
Nb3 O14 V1 93.9(4) . .
Nb1 O15 Na3 137.2(6) . .
Nb3 O16 Nb6 119.5(4) . .
Nb3 O16 K1 98.4(4) . .
Nb6 O16 K1 98.5(4) . .
Nb3 O17 Na4 139.4(6) . .
Nb4 O19 Nb1 119.7(4) . .
Nb4 O19 V1 92.0(4) . .
Nb1 O19 V1 93.7(4) . .
Nb7 O20 Nb2 120.3(5) . .
Nb7 O20 V2 93.3(4) . .
Nb2 O20 V2 93.5(4) . .
Nb5 O22 Nb6 119.2(4) . .
Nb5 O22 V2 92.3(4) . .
Nb6 O22 V2 94.6(4) . .
Nb6 O24 Nb6 150.3(7) 6_565 .
Nb6 O24 K1 103.1(4) 6_565 .
Nb6 O24 K1 103.1(4) . .
V1 O25 Na2 176.1(9) . .
K1 O1W K2 104.9(4) . 1_556
Na3 O26W K1 91.3(9) 1_556 .
Na4 O22W Na2 130.3(13) . 2_557
Na1 O21W Na1 108(3) 5_557 .
O15W O16W Na1 51(3) 7_557 7_557
O16W O15W Na1 100(4) 7_557 .
Na5 O14W K2 91(2) . 7_557
N3 C1 C6 106.6(17) . .
N1 C2 C5 107.2(16) . .
N2 C3 C4 107.5(15) . .
N4 C4 C3 107.4(18) . .
N5 C5 C2 107.3(14) . .
C1 C6 N6 111.2(15) . .
C2 N1 Cu1 107.6(10) . .
C3 N2 Cu1 110.3(12) . .
C1 N3 Cu2 109.5(10) . .
C4 N4 Cu1 108.6(10) . .
C5 N5 Cu1 109.0(11) . .
C6 N6 Cu2 107.7(10) . .
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
Nb1 O15 1.774(9) .
Nb1 O7 1.945(8) .
Nb1 O12 1.962(6) .
Nb1 O2 2.015(8) .
Nb1 O19 2.019(9) .
Nb1 O5 2.440(8) .
Nb1 V1 3.055(4) .
Nb1 K2 3.756(5) .
Nb2 O18 1.781(10) .
Nb2 O7 1.932(9) .
Nb2 O11 1.955(6) .
Nb2 O9 2.018(9) .
Nb2 O20 2.036(10) .
Nb2 O4 2.427(9) .
Nb2 V2 3.066(5) .
Nb2 K2 3.835(5) .
Nb3 O17 1.754(9) .
Nb3 O3 1.939(4) .
Nb3 O16 1.965(9) .
Nb3 O1 2.016(8) .
Nb3 O14 2.016(9) .
Nb3 O8 2.432(8) .
Nb3 V1 3.052(5) .
Nb3 K1 3.771(5) .
Nb4 O6 1.764(12) .
Nb4 O1 1.975(9) 6_565
Nb4 O1 1.975(9) .
Nb4 O19 1.986(9) 6_565
Nb4 O19 1.986(9) .
Nb4 O5 2.418(11) .
Nb4 V1 2.991(4) 6_565
Nb4 V1 2.991(4) .
Nb5 O10 1.762(9) .
Nb5 O2 1.972(8) .
Nb5 O9 1.983(8) .
Nb5 O22 1.984(9) .
Nb5 O14 2.003(9) .
Nb5 O8 2.383(8) .
Nb5 V1 2.972(4) .
Nb5 V2 2.991(5) .
Nb6 O21 1.782(10) .
Nb6 O24 1.941(3) .
Nb6 O16 1.965(9) .
Nb6 O13 2.015(9) .
Nb6 O22 2.029(10) .
Nb6 O8 2.436(8) .
Nb6 V2 3.079(5) .
Nb6 K1 3.774(5) .
Nb7 O23 1.797(13) .
Nb7 O20 1.966(10) 6_565
Nb7 O20 1.966(10) .
Nb7 O13 1.977(9) .
Nb7 O13 1.977(9) 6_565
Nb7 O4 2.394(12) .
Nb7 V2 3.013(5) .
Nb7 V2 3.013(5) 6_565
Cu1 N2 1.988(13) .
Cu1 N4 1.993(13) .
Cu1 N1 2.015(12) .
Cu1 N5 2.014(15) .
Cu1 O10 2.377(9) .
Cu1 Na5 2.81(2) .
Cu2 N6 1.993(14) 6_565
Cu2 N6 1.993(14) .
Cu2 N3 2.004(13) .
Cu2 N3 2.004(13) 6_565
Cu2 O6 2.334(13) .
V1 O25 1.598(11) .
V1 O2 1.930(9) .
V1 O1 1.937(10) .
V1 O14 2.158(11) .
V1 O19 2.167(11) .
V2 O26 1.399(14) .
V2 O9 1.917(10) .
V2 O13 1.962(10) .
V2 O22 2.158(11) .
V2 O20 2.172(12) .
Si1 O5 1.639(12) .
Si1 O8 1.649(9) 6_565
Si1 O8 1.649(9) .
Si1 O4 1.651(12) .
K1 O1W 2.787(14) 6_565
K1 O1W 2.787(14) .
K1 O3 2.810(14) .
K1 O24 2.828(14) .
K1 O2W 2.84(2) .
K1 O16 2.945(10) 6_565
K1 O16 2.945(10) .
K1 O26W 3.14(3) .
K1 O26W 3.14(3) 6_565
K1 Nb3 3.771(5) 6_565
K1 Nb6 3.774(5) 6_565
K2 O1W 2.790(14) 1_554
K2 O1W 2.790(14) 6_564
K2 O3W 2.83(4) .
K2 O7 2.836(10) .
K2 O7 2.836(10) 6_565
K2 O12 2.908(13) .
K2 O11 3.041(15) .
K2 O14W 3.25(7) 4_557
K2 O14W 3.25(7) 7_557
K2 Nb1 3.756(5) 6_565
K2 Nb2 3.835(5) 6_565
Na1 O15W 2.14(6) .
Na1 O15W 2.14(6) 2_557
Na1 O21W 2.17(4) 5_557
Na1 O21W 2.17(4) .
Na1 O16W 2.72(6) 7_557
Na1 O16W 2.72(6) 8_455
Na1 Na1 3.50(3) 5_557
Na2 O22W 2.73(4) 2_557
Na2 O25 2.778(19) .
Na2 O13W 2.86(9) .
Na2 Na2 2.86(4) 2_557
Na3 O15 2.712(19) .
Na3 O27W 2.81(3) .
Na3 O4W 2.96(3) 1_554
Na3 O26W 2.99(4) 1_554
Na3 K1 4.38(2) 1_554
Na4 O22W 2.67(4) .
Na4 O17 2.744(19) .
Na5 O14W 2.41(7) .
Na5 O25W 2.85(3) 7_558
Na5 K2 4.06(2) 7_557
O3 Nb3 1.939(4) 6_565
O4 Nb2 2.427(9) 6_565
O5 Nb1 2.440(8) 6_565
O11 Nb2 1.955(6) 6_565
O12 Nb1 1.962(6) 6_565
O24 Nb6 1.941(3) 6_565
O1W K2 2.790(14) 1_556
O4W Na3 2.96(3) 1_556
O26W Na3 2.99(4) 1_556
O25W Na5 2.85(3) 7_558
O22W Na2 2.73(4) 2_557
O21W Na1 2.17(4) 5_557
O17W O17W 0.98(9) 2_556
O16W O15W 1.36(7) 7_557
O16W Na1 2.72(6) 7_557
O15W O16W 1.36(7) 7_557
O14W K2 3.25(7) 7_557
C1 N3 1.45(2) .
C1 C6 1.47(2) .
C2 N1 1.47(2) .
C2 C5 1.49(2) .
C3 N2 1.48(2) .
C3 C4 1.51(3) .
C4 N4 1.46(2) .
C5 N5 1.48(2) .
C6 N6 1.50(2) .
